# The effect of production variables on the strength of brass/Sn-Pb-Sb solder joints: A statistical...

Embed Size (px)

### Transcript of The effect of production variables on the strength of brass/Sn-Pb-Sb solder joints: A statistical...

JOURNAL OF MATERIALS SCIENCE 29 (1994) 1731-1738

The effect of production variables on the strength of brass/Sn-Pb-Sb solder joints: a statistical analysis

M. EVANS Department of Materials Engineering, University College Swansea, Swansea, SA2 8PP, UK

Tomlinson and Cooper's data on solder joint strength have been used to illustrate the additional benefits, in terms of useful results, that can be obtained from the application of stepwise regression techniques to production process data. This technique provides extra quantitative information in three main areas. First, those production variables of importance can be identified and the exact effect of such variables on joint strength determined. Secondly, linear versus non-linear association between such production variables and joint strength can be tested. Finally, the degree and significance of interaction effects can be estimated. Using this stepwise regression technique it was found, contrary to Tomlinson and Cooper's paper, that the relationship between strength and antimony content was, in all cases, non-linear, whilst all other relationships were linear. The significant main effect variables were furnace cooling, cooling time and antimony content with the latter being the most important explanatory variable. However, the effects of these and other interaction explanatory variables were not minor as Tomlinson and Cooper suggest. Important interaction effects were also identified particularly so between gap size and antimony content.

1. In troduc t ion Statistical techniques can be useful in helping to identify those processes controlling the quality of manufactured items. With reference to data published by Tomlinson and Cooper [1] on solder joint strength, the present work sought to illustrate the nature of the additional information that can be ob- tained from the application of simple stepwise regres- sion procedures. Tomlinson and Cooper's paper was chosen because it provides a particularly good illus- tration of the extra useful information that can be obtained through use of this statistical technique.

Tomlinson and Cooper [1] accumulated a moder- ate data set to analyse the effects of certain production variables on the strength of brass/Sn-Pb Sb solder joints. Tables and simple line graphs were the methods chosen by the authors to identify those production variables which controlled the strength of the solder joint. (Their tables are reproduced here in the Appen- dix). Four production variables were examined: solder time (min), percentage content of antimony, joint gap (mm), and cooling method. From such an analysis the authors concluded that "for any solder composition the effect of these production variables is relatively small" and "overall the effect of cooling is small and the effect of joint gap in the range 0.05-0.2 mm has only a minor effect". From the way in which the separate lines in Figs 1 and 3 rotate [-1] they conclude that interaction effects between production variables are present in determining joint strength.

Given the chosen methods of analysis, it is not

surprising that Tomlinson and Cooper summarized their results in this very qualitative fashion. This present paper illustrates how stepwise regression tech- niques can be used in conjunction with the above- mentioned graphical methods to obtain the following additional diverse, detailed and precise information.

(a) Those production variables that contribute sig- nificantly (in a statistical sense) to joint strength can be found. Further, for those variables found to be signi- ficant, their precise effect on strength can be obtained as can their contribution to the variation in joint strength.

(b) The functional relationship existing between joint strength and the production variables can be ascertained. Tests for linear versus non-linear forms can be undertaken. Indeed a graphical plot of strength against solder time (Fig. 1 [1]) is not sufficient in- formation for determining whether or not the relation- ship is linear.

(c) Those variables that interact and the precise nature of this interaction in determining joint strength can be identified. Graphs alone cannot provide such quantitative detail.

The remainder of the paper illustrates the methods used to obtain this extra information, and the implica- tions that can be drawn from the results.

2. Methodology The methodology employed here has been referred to in the econometrics literature as Hendrification. This

0022-2461 �9 1994 Chapman & Hall 1731

stems from work done by Hendry on dynamic model-. ling. Hendry [-2] suggests that it is always better to start off with a general model and then simplify that model by testing for parameter restrictions. Such tests are termed specification tests, but a simplified model must also pass mis-specification tests, which test the validity of the least squares assumptions about the regression residuals. Specifically, specification tests look for parameter restrictions of the form 13~ = 0, whilst mis-specification tests, analyse the residuals for normality, constant variance and independence.

In applying this approach to data on production variables and joint strength, we come across a number of data constraints. Tomlinson and Cooper look at four production variables: they are soldering time (rain), joint gap (mm), percentage of antimony in joints, and cooling method. Four such cooling meth- ods were analysed: water-quenched (WQ), oil-quen- ched (OQ), air-blown (AB), and furnace-cooled (FC). The cooling times for each were respectively 5 s, 1, 5 min and 6 h. Shear strength (MPa) of the joint was also measured.

To be completely general, all four production vari- ables should be included in a single regression. But as Appendix 1 shows, the way in which the data were collected prevents this. However, three separate re- gressions can be constructed with the first containing antimony and soldering time, the second antimony

Y~ =

where OQ = 1 if oil quenched, 0 otherwise. AB = 1 if air blown, 0 otherwise. FC = 1 if furnace cooled, 0 otherwise. ~'~ ~ N [0, r P = 1-11 variables, and N = 48 observations on Y.

This model breaks down into four separate equa- tions, one for each type of cooling.

Water quenched: here OQ = AB = FC = 0, so

Y~ = 80 + 6~Sb~ + 626b~ 2 + c~ (2b)

Oil quenched: here OQ = 1, AB = FC = 0, so

Y; = [60 + ks] + [61 + 56] Sbi

-~- [-52 + 59" ] Sb] + 8'~ (2c)

Air blown: here AB = 1, OQ = FC = 0, so

Y, = I-So + 6~3 + [6, + 6 d S b ,

+ [62 + 5,o] Sb 2 + 8', (2d)

Furnace cooled: here FC = 1, AB = OQ = 0, so

Yi �9 = (6 o + 55) + [6 a +58]Sb i

+ [52 + 6~l]Sb ~ + 1r i (2e)

Water quenching is the bench mark in Model 2 so that the other types of cooling either shift the quadratic in Equation 2b up or down (e.g. So to (So + 63)), and/or alter the slope (e.g. 6, to (61 + 86)) and/or alter the degree of curvature (e.g. 52 to (62 + 69) ).

Model 3

Main effects Interaction effects ( - A 2 ~ r A % + ~lSb~ + ~2Sb 2 + %GPI + ~4GP~ + %Sb~GP~ + ~6SbiGP 2 + ~TSb~GP~ + %Sb~GP~a+ c'[ (3)

and cooling method and the third antimony and gap size. Each can be made general by including pow- ered terms and all interaction variables. Following Mendenhall and Sincich [3] we take as our general specification a "complete factorial model", of which

F =

there exist three, given the nature of the data set at hand.

Model 1

Main effects Interaction effects .A ^

Yi = ~B 0 + B 1T , + B2Sb ~ + B3T~ 2 + B4Sb~'+ "BsT~Sb , + B6T, Sb 2 + BTTZ~Sbi + BsT~2SbF+ e,

where Y~ is the ith reading on strength, T~ the ith reading on solder time, Sb~ the percentage antimony content, and 8 i ~ N [0, cy~]. P = 1-8 explanatory variables, and N = 48 observations on Y.

Model 2

where GPi is the ith value on gap size, c'i' ~ N [0, cr~], P = 1-8 explanatory variables, with N = 45 readings only.

The stepwise procedure now runs as follows. First we estimate the general Equations 1-3, and construct the following F test for the omission of each Jth variable

[SSRI-X,, X2, X,_ 1, X, + 1, " " , X,] - SSR[X,, X2, . . . , X , ] ]

[MSR[X,, X2, -.-, Xp] ] (4)

This has an F distribution with l and N-P-1 degrees of freedom. For Models 1 and 3, P = 8, and for Model 2, P - 11. X I to X e are the P explanatory variables.

(1)

Thus SSR[X1, Xz, Xj_I,Xj+I, Xp] is the sum of squared residuals obtained from a regression with all P explanatory variables except X j . MSR[Xt, X2,-.-,

Main effects A

Yi = 80 + '~lSbi + 628b 2 -t- 630 Q -b 6,AB + 65FC'

Interaction effects

( "% 2 "~ ; + 66Sb~O Q + 67Sb~AB + 6sSb~FC + 89Sb]OQ + 61oSb~AB + 6~ISb~FC + ai (2a)

1732

Xv] is the mean square error of a regression with all P explanatory variables.

Variables are deleted one step at a time, until no more variables can be deleted. Only variables which have low F values will be deleted, as the removal of such variables does not significantly raise the un- explained variation, SSR. In particular, only variables with F values below the critical value at the 10% level of significance, Fr are dropped.

Once all tests of specification have been carried out, so that no insignificant variables remain, the following three tests of mis-specification are carried out.

1. Form the regression

s = P lg ( i - 1 ) + P2s + "" + P6E(i-6)

P

+ xj + z , (5) ( j= 1)

where Z~ ~ N [0, ey~]. If there is no serial correlation over this range of order, then the value of R 2, (percent- age variation in a~ explained by its own past values and all significant X~ variables), from this regression should be close to zero. In fact, Breusch [4] has shown that the statistic Kz = R 2 • N , where N is the number of observations on ~, follows a %2 distribution with six degrees of freedom, under the null hypothesis of inde- pendence, i.e. under the null P~ = P2 . . . . . P6 = 0.

2. Form the regression

e~ z = X o + ;L~X~ + XzX ~ + -.-

+ X2e-1Xp + X2e X2 + Wi (6)

W~ ~ N [0, c%]. ~ has constant variance if only k o is

significant. That is, the R 2 value from this equation should be close to zero. White [5] has shown that the statistic K2 = R 2 X N , follows a Z 2 distribution with 2P degrees of freedom.

3. Jarque and Bera [6] have shown that the fol- lowing statistic has a )(2 distribution with 2 degrees of freedom under the null hypothesis of normally dis- tributed residuals

- 6 SK2 + EK2 (7)

where S K is a measure of skewness and E K is a measure of kurtosis in the residues.

The correct simplified model is one in which no more variables can be deleted by the above F test, and one which passes the KI to K 3 tests of mis-specifica- tion. Only if the model passes such mis-specification tests, can we use the standard F tests of significance in the simplified model. Least square estimates of para- meter variances will be invalid in the presence of non- normality, auto-correlation and heteroscedasticity.

All-regressions were carried out using the Minitab [7] package.

3. R e s u l t s a n d d i s c u s s i o n The main results obtained from applying the above procedure on Tomlinson and Cooper's data are shown in Tables I - I I I and Figs 1 3. Table I shows the results of the analysis when soldering time and anti- mony are the two explanatory variables. Step 1 shows

28

26 i 22 t ' -

t -

2 0 - - I11 t ' -

0 ' 3

1 8 - -

1 6 - -

14

0

O

0 % Sb

[ ] 5% Sb

Model ~ 3 % Sb ~ Model

Model A 10 % Sb ~ Model

A

A

I t I I B 10 15 20 25

Time (min)

Figure 1 Effect of soldering time at 300 ~ on the shear strength of brass/Sn-Pb-Sb joints. Joint gap, D.17 mm; cooled by blown air.

1733

24 .0 ~:~ W Q ~'~=~=~:~'~=~;~:~ Model [ ] OQ - - Model ZX AB Model

2 2 . 2

a_ 2 0 . 4

133 C

1 8 . 6 - -

1 6 . 8 - -

1 5 . 0

-2

ZX

"Q.

%%. ,. �9 "~%~%% \

"%%%~,. \

%'a=: zX "%..

%

1 I I I I f

0 2 4 6 8 10

Sb con ten t (%)

Figure 2 Effect of cooling method on the shear strength of brass /Sn-Pb-Sb joints. Joint gap, 0.17 mm.

12

25

23

a_ 21 -

t--

c

(./3

1 7 - -

0 % Sb Model [ ] 5 % Sb - - Model & 10 % Sb . 1 ~ Model

[]

[] []

15 I I I ~ ' ~ < 0 . 0 0 0 .05 O. 10 O, 15 0 . 2 0 0 .25

Joint gap (ram)

Figure 3 Effect of joint gap on the shear strength of brass /Sn-Pb-Sb joints, soldered at 300~ for l0 rain and cooled by blown air.

1734

T A B L E I S t e p w i s e r e g r e s s i o n for t h e ef fec ts o f s o l d e r i n g t i m e a n d a n t i m o n y on s h e a r s t r e n g t h o f b r a s s j o i n t s

P a r a m e t e r S t e p

1 2 3 4

M i s - s p e c i f i c a t i o n tes t s

C o n s t a n t 23.2 22.8 22.8 22.8

F . . . .

T i m e , T - 0.21 - 0.14 - 0.14 - 0.14

F 0.35 5.02 5.11 5.20

Sb 2.1 2.2 1.9 1.9

F 5.1 10.50 22.28 22.66

T i m e z, T 2 0.003 - - -

F 0.04 - - -

Sb 2 - 0.28 - 0.29 - 0.26 - 0.25

F 10.8 16.24 39.69 45.02

T i m e x Sb - 0.17 - 0.19 - 0.13 - 0.13

F 0.96 2.79 18.66 18.92

T i m e x Sb 2 0.021 0.023 0 .016 0 .014

F 1.7 3.13 12.82 25.10

T i m e 2 x Sb 0 .002 0.003 - -

F 0.06 0.35 -

T i m e 2 x Sb 2 - 0 .0003 0 .0004 - 0 .00008 -

F 0.21 0.52 - 0.35 -

R 2 ( % ) 85.05 85.03 84.90 84.78

cy E 1.24 1.22 1.21 1.20

F c (0.1) 2.84 2 .844 2.849 2.853

K 1 = 6.7

K 2 = 7.7

K 3 = 0.7

T A B L E I I S t e p w i s e r e g r e s s i o n for t he effects o f a n t i m o n y a n d c o o l i n g m e t h o d on s h e a r s t r e n g t h o f b r a s s j o i n t s

P a r a m e t e r S t e p

1 2 3 4 5 6 7 8

M i s - s p e c i f i c a t i o n

tes t s

C o n s t a n t 18.2 18.2 18.7 19.1 19.6 19.1 19.2

F . . . . . .

Sb 0.90 0.88 0.88 0.73 0.57 0.57 0.44

F 6.05 12.04 11.76 9.49 7.02 7.02 5.24

O Q 3.60 3.58 3.26 2.73 2.81 2.75 2.07

F 11.22 13.18 11.29 9.06 9.36 9.0 7.45

A B 2.21 2.17 1.53 1.31 1.55 1.38 1.38

F 4.2 9.24 7.78 6.05 9.0 7.95 7.84

F C 1.72 1.70 1.38 - - -

F 2.56 2.96 2.02 . . . .

Sb z - 0 . 1 0 8 - 0 . 1 0 7 - 0 , 1 1 6 - 0 . 1 1 - 0 . 0 8 9 - 0 . 0 8 5 - 0 . 0 7

F 10.18 18.92 23.72 21.16 19.01 18.06 16.97

Sb x O Q - 0.96 - 0.94 - 0.94 - 0.79 - 0.63 - 0.63 - 0.09

F 3.42 4.54 4.45 3.24 2.13 2.13 0.52

Sb x A B - 0.03 . . . .

F 0.003 - - -

Sb x F C - 0 .94 - 0.93 - 0.93 - 0.48 - -

F 3.31 4.41 4.33 2.25 - - -

Sb 2 x O Q 0.075 0 .074 0.083 0 .072 0 ,056 0 .052 -

F 2.46 3.17 4.04 3.10 1.90 1.69

Sb 2 x A B - 0 .016 - 0 .019 . . . .

F 0.12 1,88

Sb 2 x F C 0.085 0.083 0.093 0.06 0.01

F 3.13 4.08 5.06 2.99 1.06 - -

R 2 ( % ) 69.36 69.36 67.8 66.08 64.13 63.19 61.66

~ 1.35 1.33 1.34 1.36 1.38 1.38 1.39 F c (0.1) 2.858 2.862 2.867 2.871 2.876 2.88 2.884

19.3

0.42

4.88

1.65 11.36

1.38

7.90

- 0 .07

17.22

61.20

1.39 2.889

K 1 = 1.1

K 2 = 4.4

K 3 = 0.1

the general regression given by Equation 1. The vari- able with the smallest F value below the critical value of Fc = 2.84, is the square of time, T 2. This variable is then dropped for the second step regression. In all, four steps are required to remove all insignificant variables at the 10% level. At the 10% level of signifi- cance the model passes all three tests of mis-specifica-

tion. The simplified model, in which all variables are significant at the 10% level of significance is therefore

Y~ = 22.8 - 0.14T~ + 1.9Sbi - 0.25Sb 2

- 0 . 1 3 TzSbi + 0.014 T~Sb 2 + ~ (8)

From this we can draw the following conclusions. (a) Joint strength is a linear function of soldering

1735

T A B L E III Stepwise regress ion for the effects of a n t i m o n y a n d j o i n t g a p on the shea r s t r e n g t h of b ra s s j o in t s

P a r a m e t e r Step

1 2 3 4

Mis-spec i f ica t ion tests

C o n s t a n t 21.4 21.3 20.8 20.6

F - - -

Sb 0.71 0.78 0.84 0.89

F 0.38 3.57 5.62 8.24

G a p , G P - 13.1 - 11.9 - 2.0

F 0.10 0.10 0.09 -

Sb / - 0 .139 - 0 .146 - 0 .146 - 0.149

F 1.61 29.2 29.8 33.4 G a p z, G P 2 44 40 - -

F 0.07 0.07 -

Sb • G a p 8.8 7.3 6.1 5.9

F 0.17 1.59 2.72 2.89

Sb • G a p z - 59 53 - 48 - 50

F 0.49 4.19 6.97 8.07 G a p x Sb 2 - 0.1 - -

F 0.005 Sb 2 x G a p z 2.7 2.1 2.1 2.2

F 0.11 2.69 2.72 3.84

R2(%) 74.06 74.06 74.01 73.94

o~' 1.42 1.40 1.39 1.37

F~ (0.1) 2.858 2.862 2.867 2.871

K 1 = 9.9

K z = 6.1

K 3 = 0.3

T A B L E IV E x p l a i n e d va r i a t i ons for M o d e l 1, s implif ied

T i 24 .92%

Sbi 40 .03%

Sb~ 9 .89%

TiSb i 0 .84% rgSb~ 2 9 .10%

All 84 .78%

time but a non-linear function of antimony content. This is true at the 10% level of significance.

(b) The variables in Equation 8 jointly explain 84.78% of the total variation in joint strength. 15.2% of the variation remains unexplained. Table IV gives a detailed breakdown of this explained variation. Thus antimony is by far the more important of the explan- atory variables, followed by solder time, and S b 2. That is, the main effects part of the model dominates.

Equation 8 suggests that a one percentage point increase in antimony will induce a 1.65 point MPa increase ( 1 . 9 - 0.25 = 1.65), all other things being equal. In turn, an increase in soldering time of 1 min induces a 0.14 point MPa decrease, all other things equal. These figures are on the average estimates.

(c) From Table IV, significant interactions take place between time and antimony so as to account for 9.94% of the total variation in joint strength. All percentage figures in Table IV are significant at the 10% level of significance. Thus if solder time goes up by 1 rain and antimony by one percentage point, there will be a fall in MPa of 0.116 units above that predic- ted by the main effects shown in (b) above. This is true on average. This explains why, in Fig. 1 below, the four linear lines rotate as the antimony content is varied. The four linear lines simply plot Equation 8 when Sb = 0%, 3%, 5% and 10%, respectively, and ~i = O.

1736

Table II shows the results of the analysis when antimony and cooling method are the two explan- atory variables. Step 1 shows the general model given by Equation 2a. In this regression the parameter with the smallest F value below the critical value, F c = 2.858, at the 10% level is Sb • AB. This variable is then dropped for the second step regression. In all, eight steps are required to remove all insignificant variables at the 10% level of significance. Again at the t0% ievel the simplified model passes all three mis- specification tests.

The simplified model, in which all variables are significant at the 10% level is, therefore

Y~ = 19.3 + 0.42Sb~ + 1.65OQ

+ 1.38 AB - 0.07 Sb~ + ~'i (9a)

From this we can draw the following conclusions. (a) Joint strength is a non-linear function (quad-

ratic) of antimony content. This is true at the 10% level of significance.

(b) From Equation 9a we have

Yi = 19.3 + 0.42Sb~ - 0.07Sb 2 + ~'~ (9b)

when water quenching is used.

Y~ = 20.95 + 0.42Sb~ - 0.07Sb~ + a'~ (9c)

when oil quenching is used.

Y~ = 20.68 + 0.42Sb~ - 0.07Sb~ + ~'~ (9d)

when air-blown cooling is used. At the 10% level of significance Equations 9b-d are significantly different. Excluding furnace cooling, changes in cooling method shift the quadratic relationship between strength and antimony content upwards in a parallel fashion. How- ever, no matter what type of cooling is used, every one percentage point rise in antimony will add to MPa

TABLE V Explained Variation for Model 2, simplified

Sbl 32.52% Sb~ 15.51% OQ 6.02% AB 7.15%

All 61.2"/o

TABLE VI Explained variation for Model 3, simplified

Sbl 35.55% Sb{ 28.24% Sb~ x GP i 4.66% Sbi x GP~ 2.93%

Sb~ x GP~ 2.56%

All 73.94%

some 0.28 units. That is

dY = 0.42 - 0.14Sb (10)

dSb

This holds on average. The variables in Equation 9a explain 61.2% of the

variation in joint strength. Some 38.8% of the varia- tion remains unexplained. Table V shows a more detailed breakdown of this explained variation. Sb~ and its square are by far the most important explan- atory variables. However, the methods of cooling are capable of explaining some 13.17% of the variation in joint strength. This is significant at the 10% level.

(c) Equations 9b-d highlight the fact that no signi- ficant interactions take place. The cooling method simply alters the constant term in Equation 9a. That is, changes in the cooling method shift the quadratic in strength-antimony space in a parallel manner. This is shown in Fig. 2 in which Equations 9a-d are plotted for ~'i = 0.

Table III shows the results of the analysis when antimony and gap size are the explanatory variables. Step 1 shows the general model given by Equation 3. The variable with the smallest F value below the critical value of F~ = 2.858, is GP x Sb 2. This variable is then dropped for the second step regression. In all, four steps are needed to remove all insignificant vari- ables at the 10% level. At this 10% level of significance the simplified model passes all three mis-specification tests. The simplified model in which all variables are significant at the 10% level is given by

Yi = 20.6 + 0.89Sb~ - 0.149Sb 2 + 5 .9SblxGPi

- 50Sb~x GP~ + 2.2Sb~GP 2 + e' i' ( 1 1 )

From this we can draw the following conclusions. (a) Joint strength is a non-linear function (quad-

ratic) of antimony content, but a linear function of gap size. Thus the curves shown in Fig. 3 of Tomlinson and Cooper's article are not curves at all, at the 10% level of significance. Evidence for divergence from a straight line is not present in the data.

(b) The variables in Equation 11 jointly explain 73.94% of the total variation in joint strength. 26.06% of the variation in joint strength remains unexplained. Table VI contains a further breakdown of this ex- plained variation. Again Sb and Sb 2 are by far the most important explanatory variables. The main ef- fects part of the model dominates. Gap size as a variable on its own does not significantly affect joint strength, although it does have an interaction effect with antimony. Ignoring such interaction, an increase of one percentage point in antimony adds 0.592 units

to the MPa measure. That is

dY

dSb - 0.89 - 0.298Sb (12)

These are, on average, estimates. (c) Table VI shows that significant interaction ef-

fects take place between Sb and GP, Sb and GP 2 and Sb 2 and GP 2 on strength. All such interactions help explain 10.15% of the variation in joint strength. Through such interactions a 0.1 mm rise in gap size with a one percentage point rise in antimony will add 0.112 MPa to joint strength on average. This helps explain why in Fig. 3 the three linear lines rotate as antimony varies. These three linear lines simply plot Equation 11 when Sb = 0%, 5% and 10%, respect- ively, with a' i' = O.

4. Conclusion The results illustrate that the percentage content of antimony is the most important production variable determining joint strength. However, the effects of other variables are far from minor. In Model 1, solder time helps explain nearly a quarter of the variation in joint strength, whilst in Model 2, some 13% of joint

T A B L E VII Effect of soldering time at 300~ on the shear strength of brass /Sn-Pb-Sb joints. Joint gap 0.17 mm; cooled by blown air

Sb (%) Time (min) Shear strength (MPa)

1 2 3 Average

0 5 22.9 21.5 20.6 21.6 0 10 22.8 21.7 20.6 21.7 0 15 19.6 19.4 21.7 20.3 0 20 19.4 21.3 20.1 20.3 0 60 16.3 - - 16.3

3 5 26.7 24.4 26.2 25.7 3 10 22.1 22.9 21.7 22.2 3 15 20.1 18.7 22.1 20.3 3 20 19.1 17.1 18.7 18.3 3 60 16.1 - 16.1

5 5 24.4 21.3 23.3 23.0 5 10 22.3 22.1 19.4 21.3 5 15 19.6 21.3 18.3 19.8 5 20 18.6 15.8 18.1 17.5 5 60 15.9 - 15.9

10 5 15.2 17.6 17.1 16.7 10 10 17.1 t7.3 16.3 16.9 10 15 16.3 17.4 15.2 16.3 10 20 16.4 15.2 15.5 15.7 10 60 15.7 - 15.7

1737

strength variation is explained by cooling methods. In Model 3 interaction effects were shown to be very important. Thus, whilst gap size on its own is irrel- evant, its interaction with antimony helps explain 10% of the variation in joint strength. Finally, joint strength was shown to be a linear function of solder time and gap size, not non-linear as Tomlinson and Cooper suggest, and a non-linear function of anti- mony content.

These simple statistical procedures have helped quantify and identify the important and not so im- portant production variables and, in some cases, even modified some of Tomlinson and Cooper's conclu- sions. It is clear that a whole wealth of extra informa- tion can be gleamed from the authors' data with the use of this simple regression procedure.

Acknowledgements The author thanks W. Tomlinson and G. Cooper for use of their data, and Mrs M. Rees for typing this paper.

T A B L E IX Effect of joint gap on the shear strength of b ra s s /Sn-Pb-Pb-Sb joints soldered at 300 ~ for 10 min and cooled by blown air

Sb (%) Gap (mm) Shear strength (MPa)

1 2 3 Average

0 0.05 19.6 23.0 20.4 21.0 0 0.07 18.5 20.8 21.9 20.4 0 0.10 19.0 21.9 21.1 20.7 0 0.15 22.3 19.0 20.0 20.4 0 0.20 17.8 22.9 20.9 20.5

5 0.05 20.1 23.5 24.8 22.8 5 0.07 22.9 22.5 19.8 21.7 5 0.10 22.5 22.9 21.9 23.4 5 0.15 20.6 20.5 23.8 21.7 5 0.20 19.0 20.5 18.7 19.4

10 0.05 16.0 16.3 17.5 16.6 10 0.07 18.7 17.1 17.8 17.9 10 0.10 19.0 17.1 16.7 17.6 10 0.15 17.6 17.0 17.1 17.3 10 0.20 t6.2 15.2 15.0 15.5

T A B L E V I I I Effect of cooling rate after soldering time at 300 ~ for 10 rain on the shear strength of brass /Sn-Pb Sbjoints. Joint gap = 0.17 mm; WQ = water quenched, OQ = oil quenched, AB = air

blown, FC = furnace cooled

Sb (%) Cooling Shear strength (MPa) method

1 2 3 Average

0 WQ 17.6 19.5 18.3 18.5 0 OQ 20.0 24.3 21.9 20.1 0 AB 18.3 19.8 22.9 20.3 0 FC 19.4 19.8 20.3 19.8

3 WQ 18.6 19.5 19.0 19.0 3 OQ 20.0 20.9 20.4 21.1 3 AB 21.7 22.9 22.1 22.2 3 FC t9.0 20.9 19.9 19.7

5 WQ 22.3 19.5 20.5 20.8 5 OQ 20.9 22.9 20.6 21.5 5 AB 22.9 19.7 21.6 21.4 5 FC 19.6 16.4 20.5 18.8

10 WQ 15.2 17.1 16.6 16.3 10 OQ 16.4 19.0 18.1 17.8 10 AB 15.8 17.3 17.1 16.8 10 FC 16.4 17.6 17.6 17.2

Appendix Tables VII-IX give the original data published by Tomlinson and Cooper. As can be seen, three MPa observations are made against two explanatory vari- ables in each table. Thus only two such variables can be included in any one regression equation

References 1. W. J . T O M L I N S O N and G. A. COOPER, J. Mater. Sci. 21

(1986) 1730-1734. 2. D. F. HENDRY, in "Economic Modelling", edited by P.

Omerod (London, 1979) Ch. 9. 3. w. M E N D E N H A L L and T. SINCICH, "Statistics for the

Engineering and Computer Sciences," 2nd Edn (Maxwell- Macmillan, London, 1989) Ch. 12.

4. T .S . BREUSCH, Austral. Econom. Papers 17 (1978) 334 355. 5. H. WHITE, Econometriea 48 (1980) 817-838. 6. M. C. JARQUE and K. A. BERA, Eeonom. Lett. 6 (1980)

255-259. 7. MINITAB Reference Manual (Minitab Inc., State College, PA,

1989).

Received 20 August 1992 and accepted 27 September 1993

1738